advertisement

CHAPTER 3: Crystal structures and properties ISSUES TO ADDRESS... • How do atoms assemble into solid structures? (for now, focus on metals) • How does the density of a material depend on its structure? • When do material properties vary with the sample (i.e., part) orientation? 1 Energy and packing • Non dense, random packing • Dense, regular packing Dense, regular-packed structures tend to have lower energy. 2 Materials and packing Crystalline materials... • atoms pack in periodic, 3D arrays • typical of: -metals -many ceramics -some polymers crystalline SiO2 Adapted from Fig. 3.18(a), Callister 6e. Noncrystalline materials... • atoms have no periodic packing • occurs for: -complex structures -rapid cooling "Amorphous" = Noncrystalline noncrystalline SiO2 Adapted from Fig. 3.18(b), Callister 6e. 3 Metallic crystals • tend to be densely packed. • have several reasons for dense packing: -Typically, only one element is present, so all atomic radii are the same. -Metallic bonding is not directional. -Nearest neighbor distances tend to be small in order to lower bond energy. • have the simplest crystal structures. We will look at three such structures... 4 Simple Cubic (SC) structure • Rare due to poor packing (only Po has this structure) • Close-packed directions are cube edges. • Coordination # = 6 (# nearest neighbors) (Courtesy P.M. Anderson) 5 Atomic Packing Factor (APF) • APF for a simple cubic structure = 0.52 Adapted from Fig. 3.19, Callister 6e. 6 Body Centered Cubic (BCC) structure • Close packed directions are cube diagonals. --Note: All atoms are identical; the center atom is shaded differently only for ease of viewing. • Coordination # = 8 Adapted from Fig. 3.2, Callister 6e. (Courtesy P.M. Anderson) 7 Atomic Packing Factor: BCC • APF for a body-centered cubic structure = 0.68 R Adapted from Fig. 3.2, Unit cell contains: 1 + 8 x 1/8 = 2 atoms/unit cell a Callister 6e. 8 Face Centered Cubic (FCC) structure • Close packed directions are face diagonals. --Note: All atoms are identical; the face-centered atoms are shaded differently only for ease of viewing. • Coordination # = 12 Adapted from Fig. 3.1(a), Callister 6e. (Courtesy P.M. Anderson) 9 Atomic Packing Factor: FCC • APF for a body-centered cubic structure = 0.74 a Unit cell contains: 6 x 1/2 + 8 x 1/8 = 4 atoms/unit cell Adapted from Fig. 3.1(a), Callister 6e. 10 FCC stacking sequence • ABCABC... Stacking Sequence • 2D Projection A B B C A B B B A sites C C B sites B B C sites • FCC Unit Cell 11 Hexagonal Close-Packed (HCP) structure • ABAB... Stacking Sequence • 3D Projection • 2D Projection A sites B sites A sites Adapted from Fig. 3.3, Callister 6e. • Coordination # = 12 • APF = 0.74 12 Theoretical density, Example: Copper Data from Table inside front cover of Callister (see next slide): • crystal structure = FCC: 4 atoms/unit cell • atomic weight = 63.55 g/mol (1 amu = 1 g/mol) • atomic radius R = 0.128 nm (1 nm = 10 -7cm) Result: theoretical Cu = 8.89 g/cm3 Compare to actual: Cu = 8.94 g/cm3 14 Characteristics of Selected Elements at 20C At. Weight Element Symbol (amu) Aluminum Al 26.98 Argon Ar 39.95 Barium Ba 137.33 Beryllium Be 9.012 Boron B 10.81 Bromine Br 79.90 Cadmium Cd 112.41 Calcium Ca 40.08 Carbon C 12.011 Cesium Cs 132.91 Chlorine Cl 35.45 Chromium Cr 52.00 Cobalt Co 58.93 Copper Cu 63.55 Flourine F 19.00 Gallium Ga 69.72 Germanium Ge 72.59 Gold Au 196.97 Helium He 4.003 Hydrogen H 1.008 Density (g/cm3) 2.71 -----3.5 1.85 2.34 -----8.65 1.55 2.25 1.87 -----7.19 8.9 8.94 -----5.90 5.32 19.32 ----------- Atomic radius (nm) 0.143 -----0.217 0.114 Adapted from -----Table, "Charac-----teristics of 0.149 Selected Elements", 0.197 inside front 0.071 cover, 0.265 Callister 6e. -----0.125 0.125 0.128 -----0.122 0.122 0.144 ----------15 Densities of material classes metals • ceramics• polymers Why? Metals have... • close-packing (metallic bonding) • large atomic mass Ceramics have... • less dense packing (covalent bonding) • often lighter elements Polymers have... • poor packing (often amorphous) • lighter elements (C,H,O) Composites have... • intermediate values Data from Table B1, Callister 6e. 16 Polycrystals • Most engineering materials are polycrystals. 1 mm Adapted from Fig. K, color inset pages of Callister 6e. (Fig. K is courtesy of Paul E. Danielson, Teledyne Wah Chang Albany) • Nb-Hf-W plate with an electron beam weld. • Each "grain" is a single crystal. • If crystals are randomly oriented, overall component properties are not directional. • Crystal sizes typ. range from 1 nm to 2 cm (i.e., from a few to millions of atomic layers). 18 Single vs polycrystals • Single Crystals Data from Table 3.3, Callister 6e. (Source of data is R.W. Hertzberg, -Properties vary with direction: anisotropic. -Example: the modulus of elasticity (E) in BCC iron: Deformation and Fracture Mechanics of Engineering Materials, 3rd ed., John Wiley and Sons, 1989.) • Polycrystals -Properties may/may not vary with direction. -If grains are randomly oriented: isotropic. (Epoly iron = 210 GPa) -If grains are textured, anisotropic. 200 mm Adapted from Fig. 4.12(b), Callister 6e. (Fig. 4.12(b) is courtesy of L.C. Smith and C. Brady, the National Bureau of Standards, Washington, DC [now the National Institute of Standards and Technology, Gaithersburg, MD].) 19 Anisotropy Demo: Heating and cooling of iron wire • Demonstrates "polymorphism" The same atoms can have more than one crystal structure. 22 CHAPTER 12: Structure of ceramics ISSUES TO ADDRESS... • Structures of ceramic materials: How do they differ from that of metals? 1 CERAMIC BONDING • Bonding: --Mostly ionic, some covalent. --% ionic character increases with difference in electronegativity. • Large vs small ionic bond character: Adapted from Fig. 2.7, Callister 6e. (Fig. 2.7 is adapted from Linus Pauling, The Nature of the Chemical Bond, 3rd edition, Copyright 1939 and 1940, 3rd edition. Copyright 1960 by Cornell University. 2 Ionic bonding & structure • Charge Neutrality: --Net charge in the structure should be zero. --General form: • Stable structures: --maximize the # of nearest oppositely charged neighbors. Adapted from Fig. 12.1, Callister 6e. 3 Coordination # and ionic radii • Coordination # increases with Issue: How many anions can you arrange around a cation? Adapted from Fig. 12.4, Callister 6e. Adapted from Fig. 12.2, Callister 6e. Adapted from Table 12.2, Callister 6e. Adapted from Fig. 12.3, Callister 6e. 4 Sample calculations of radii ratios CN = 6 – Octahedral site rC rA rC rA rA 2 rC 1 rA rC rA 2 2 1 0.414 CN = 4 – tetrahedral site 2rA h 6 3 rC rA h 2 r rC rA A 6 3 rC rA rC 6 1 rA 3 rC 6 1 0.225 rA 3 Structure of compounds: NaCl • Compounds: Often have similar close-packed structures. • Structure of NaCl • Close-packed directions --along cube edges. CN = 6 (Courtesy P.M. Anderson) (Courtesy P.M. Anderson) 13 Example: Predicting structure of FeO • On the basis of ionic radii, what crystal structure would you predict for FeO? Cation Al3+ Fe 2+ Fe 3+ Ca2+ Anion O2ClF- • Answer: r cation 0.077 r anion 0.140 0.550 Data from Table 12.3, Callister 6e. 5 Example: Predicting structure of FeO • On the basis of ionic radii, what crystal structure would you predict for FeO? Cation Al3+ Fe 2+ Fe 3+ Ca2+ Anion O2ClF- • Answer: r cation 0.077 r anion 0.140 0.550 based on this ratio, --coord # = 6 --structure = NaCl Data from Table 12.3, Callister 6e. 5 AmXp structures r cation 0.100 0.8 • Consider CaF2 : r anion 0.133 • Based on this ratio, coord # = 8 and structure = CsCl. • Result: CsCl structure w/only half the cation sites occupied. • Only half the cation sites are occupied since #Ca2+ ions = 1/2 # F- ions. Adapted from Fig. 12.5, Callister 6e. 6 AmBnXp structures BaTiO3 Perovskite Ti4+ Ba2+ CN=6 CN=12 MgAl2O4 Spinels O2- Mg2+ Al3+ CN=4 CN=6 O2- Summary • Atoms may assemble into crystalline or amorphous structures • We can predict the density of a material, provided we know the atomic weight, atomic radius, and crystal geometry (e.g., FCC, BCC, HCP) • Different structures of the same material are called polymorphs; the material is said to display polymorphism • Material properties generally vary with single crystal orientation (i.e., they are anisotropic), but properties are generally non-directional (i.e., they are isotropic) in polycrystals with randomly oriented grains 23 X-RAYS TO CONFIRM CRYSTAL STRUCTURE • Incoming X-rays diffract from crystal planes. Adapted from Fig. 3.2W, Callister 6e. • Measurement of: Critical angles, qc, for X-rays provide atomic spacing, d. 20 Crystallographic directions and planes Objectives • To be able to sketch directions corresponding to indices or vice versa in a cubic crystal system • Specify Miller indices for planes drawn into a unit cell • Compute planar and linear densities Crystal systems Cubic system •3 mutually axes; a b g = 90 •3 equal edges; a = b = c (lattice constants) Cubic system is only one of seven crystal systems! (3) Cubic (2) Tetragonal (4) Orthorhombic (2) Monoclinic (1) Triclinic (1) Hexagonal (1) Rhombohedral a=b=c a=b≠c a≠b≠c a≠b≠c a≠b≠c a=b≠c a=b=c All angles = 90 All angles = 90 All angles = 90 2 angles = 90; one ≠ 90 All angles ≠; none = 90 2 Angles = 90; one = 120 All angles equal ≠ 90 Seven crystal systems are results from the arrangement of 14 different ways of arranging equivalent points in space – Bravais lattices Crystal directions • Crystal Directions – a vector - can be identified in a xyz coordinate system – 1. Choose an origin so that vector passes through it – 2. Write the coordinate of the end of the direction vector – 3. Write the coordinate of the origin of the direction vector – 4. Subtract the coordinate of the end from the coordinate from the origin – 5. Multiply all numbers by a common integer, as necessary, to reduce fractions – 6. Write the crystal direction enclosed by brackets without commas • • Generally designated by [uvw] Negatives are represented with a bar above the number z A B F y C E x D Miller Indices (crystal planes) • Crystal Planes can also be defined within a cell. – 1. Select a convenient origin for the coordinate system so that the plane does not pass through it – 2. Find the coordinate of the points where the plane intersects the 3 major axes. (If the plane does not intersect a particular axis, the intercept is infinity!) – 3. Take the reciprocal (inverse) of the intercepts – 4. The plane indices are the final numbers obtained • Generally designated as (h k l) also called Miller indices z B A C y D x Family of directions Directions in cubic system [100], [010], [001], [100], etc. are equivalent The family is represented by <100> All combinations of [123] directions regardless of signs are also equivalent – they are part of the <123> family All combinations of (111) planes, regardless of signs are equivalents The family is represented by {111} Not true in non-cubic systems!!! Planes and direction relationships Make a note, we will be using this later Planes and directions that share the indices are perpendicular [hkl] is perpendicular to (hkl) (h.u+kv+l.w) Cosine q = (h2+k2+l2)1/2.(u2+v2+w2)1/2 Not true in non-cubic systems!!! q Linear density • We saw that many properties depended on crystal directions Linear density = Number of atoms centered on a segment Length of segment LD110 = 2 atoms 4R ;(m)-1 Planar density Properties of crystals can be dependent on the specific plane (chemical, mechanical, magnetic etc.) Planar density = Number of atoms centered on a plane 4R/√2 Area of plane Example: Find FCC (lead) with Pb radius of 1.750 Å –PD110 = 2atoms/8R2√2; (m)-2 –PD111 = 2atoms/4R2√2; (m)-2 4R/2√3 4R Both directions and planes (their densities) are important to the mechanism of slip. It is the mechanism of metal deformation!!! Use of interplanar spacing = (hkl) a (h2+k2+l2)1/2 Parallel planes of atoms Bragg’s Law: nl = 2d sin q Allows the determination of • Crystal structure • Crystal orientation • Lattice parameter • Compound identification ANNOUNCEMENTS Reading: All of Chapter 3 Core Problems: due today 2:17, 20, 22; 3:1, 13; 12: 1, 5, 25 Self-help Problems: Examples problems in text 0